Post on 22-Nov-2014
Embed Size (px)
ViscoseRecommendations for Pre-treatment,dyeing and finishing
Yohji Yamamoto viscose shirt Spring-Summer 2006
Viscose Viscose manufacture Viscose physical properties How manufacture and physical properties influence dyeing Pre-treatment Dyeing FinishingVersace viscose polo shirt
To make rayon, sheets of purified cellulose are steeped in caustic soda, dried, shredded into crumbs, and then aged in metal containers for 2 3 days. The temperature and humidity in the metal containers are carefully controlled. After ageing, the crumbs are combined and churned with liquid carbon disulphide, which turns the mix into orange-coloured crumbs known as sodium cellulose xanthate. The cellulose xanthate is bathed in caustic soda, resulting in a viscose solution that looks and feels like honey.
After the syrupy viscose solution is prepared it is forced through a spinneret into an acid bath containing sulphuric acid, sodium sulphate and, usually, Zn++ ions, causing the cellulose to be regenerated and precipitate from solution. The resulting strings or filaments are then stretched on godet wheels to strengthen them, and put into a spinning Topham box. The result is the formation of fine filaments of cellulose, or rayon.
Possible sulphur residues can generate reducing conditions destroying or changing the shade of dyestuffs
Viscose manufactureCross-section Longitudinal-section After initial skin formation, the core of the fibre decomposes, hardens and shrinks. Viscose fibres are therefore characterised by an irregular, serrated skin and cross section. The skin is said to consist of many small crystalline regions. The core, on the other hand, Viscose Rayon develops a coarser crystalline structure. Differences in the ratio of skin to core impact on fibre properties and dyeing behaviour. Dye diffusion is therefore crucial to dyeing speed and extra kinetic energy is needed for dye penetration especially when swollen to its maximum by heat.
Viscose propertiesViscose has lower tenacity in both wet and conditioned state than cottonStress-strain curves of different spun fibres wet60[cN/tex]
50 40 30 20 10 0 0 2.5 5 7.5 10 12.5 14 15 17.5 20 30[Elongation %]
Polyester M odal Viscose CO
Viscose propertiesViscose has lower tenacity in both wet and conditioned state than cotton more care is necessary to prevent fabric breakages and tears in wet processing Dry and wet tenacity45 40 35 30
25 20 15 10
Cotton conditioned wet
Viscose propertiesViscose has greater elongation in both wet and conditioned state than cotton it will be stretched or distorted more under tension. Dry and wet elongation25
Cotton conditioned wet
Viscose propertiesViscose and Modal fibres are supplied in a pure state and with a higher degree of whiteness than cotton. Bleaching is only required for a full white or pastel shades. Viscose/cotton blends require bleaching baths with a reduced chemical content.Degree of whiteness (Berger)100 90 80 70 60 50 40 30 20 10
Viscose propertiesThe water retention value (swelling index) of viscose is very much higher than that of cotton. In aqueous liquors, viscose fibres tend to swell more strongly than Modal fibres or cotton. This swelling process happens very quickly and is almost complete after ten seconds at the lower temperature range. Fabrics become much more stiff when wet because the fibres are so swollen. In their swollen state, viscose fibres can become set to a certain extent. This is called hydro plasticity.
How manufacture and physical properties influence dyeingDifferent ratio of crystalline and amorphous regions compared to cotton Viscose has irregular serrated skin and cross section. Viscose loses tenacity when wet. Wet swelling increases with temperature Viscose has higher dye affinity than cotton. Inferior diffusion and penetration. More kinetic energy needed. Hot reactive dyes. More care needed to avoid damage. Very important in package dyeing. Liquor circulation should mainly be IN to OUT. OUT to IN should be < 30 seconds. Use longer L.R. than for cotton. Keep liquors above 50 C, Cool at maximum 1 C per min. Use suitable anti-crease lubricants. Mild peroxide bleach may be necessary to remove sulphur. Little preparation required. Bleaching chemicals can be reduced. Always give SOME preparation to avoid carry over of sulphur.
Swelling of fibres makes wet fabrics stiff. Swelling and heat can set creases. Viscose may contain residues of sulphur. Viscose is creamy white in colour, naturally clean. Fabrics free from natural fats and waxes, motes and seeds.
Dyes have higher substantivity and faster Use Migration dyeing techniques (at up to fixation 110 C). Add salt after dye.
Pre-treatment! Scouring and bleaching need to be mild in nature. The fabrics should always be scoured, and never put straight into dye because it is important to remove any residual sulphur to prevent dye reduction. Spinning lubricants used on viscose tend to yellow with heat, and so should be removed for best whites and bright pastels. ! The liquor ratio may need to be a little higher than for cotton, because of the higher water retention but also because of the high swelling. (Reduce jet capacity) ! Break outs are always an issue on viscose, particularly where there is lengthways tension on the fabric. Best avoided by sewing the fabric at an angle, not straight across. Use multiple "zig-zag" stitching for additional security. ! Fabrics will tend to stiffen in tight constructions so lubrication is important. There should be as little tension on the fabric as possible, because of the low wet modulus it will stretch easily and dimensional stability may never be achieved. Usually means slower turn around times and dyeing machines with winches to help the fabric into the jet, or the cigar-type machines with the fabric movement into the jet being downwards (like the Gaston County Futura or Hisaka). The more soft flow the dyeing machine the better.
Creasing and breaking of sewingsLeave small opening to allow ballooning of air to escapeSew at an angle not straight across.
Fabric delivered to dyeing machine already folded and each piece sewn at an angle to next piece, with more than one zig-zag stitching. Rope is loaded into dyeing machine without twist
Load into jet machine Only pieces of equal diameter should be sewn together
Pre-treatmentBetter base white than cotton, therefore bleaching mainly required only for full white or pastel shades. Woven fabrics Warps of viscose rayon can be sized with a variety of agents : starch based systems, polyvinyl alcohol systems or a combination of both, modified starch, starch ethers or CMC or combinations of these. Identification of the size present is important prior to deciding on a suitable desizing procedure, however, many factories will opt to use their standard cotton desize treatment : e.g. applying in the quench box of a singeing machine : pad 2 - 4 g/l amylase enzyme (Nearzim 610) 1 - 2 g/l wetting agent ( Nearfil PO )
impregnate at 60C ; pick-up 80 % ; batch minimum 4 hours - normally overnight ; wash-off.
Pre-treatmentRelax / scouring Viscose rayon fibres, unlike natural cellulosic fibres, are free from natural fats and waxes, motes and seeds, and the scouring process, therefore, need not be as severe as for cotton, and can be based on soda ash or tetra sodium pyrophosphate recipes rather than caustic soda. A typical scouring recipe on a 5 box continuous open width washing range would be : Box 1 Box 3 3 g/l Nearpon CLF 2 g/l Nearchel TMC at 95C 2 g/l Soda Ash 1 g/l Nearchel TMC Box 4 at 95C Water only at 70C Box 2 1 g/l Nearchel TMC at 95C Knitted fabric on jet or overflow machine 2 4 ml/l Lubrifil LV, Lubrifil TFS or 0.5 1 g/l Lubrifil LAF 0.5 1 g/l Nearpon BW-LF or Nearpon LF-JET 0.5 2 g/l Nearchel SA Run 20 to 30 minutes at 60-90 C 1 3 g/l Soda ash (about pH 9) Hot rinse Box 5 Water only cold
Pre-treatmentPeroxide bleach on jet or overflow machine For full white 1.0 3 ml/l Lubrifil LV or Lubrifil TFS, or 0.5 1 g/l Lubrifil LAF 2 4 g/l Nearcand OP-LF 2 6 ml/l Hydrogen peroxide 35% 0.3 0.7 % Nearoptic LNC or 0.2 0.6% Nearoptic CD-2F Run 40 minutes at 85 C Hot rinse at 60 80 C Neutralise with Nearchel MTB for 10 15 minutes at 50-60 C
If dyeing after bleaching, omit optical brightening agent, add 0.1 0.5 ml/l catalase enzyme, Neareduxol EX to same bath after neutralising with Nearchel MTB, to prevent oxidative damage to dyes by residual peroxide. There is a high risk of forming permanent creases in rope dyeing machines because viscose fibre swells and fabrics become stiff. Fabric will therefore not run well at temperatures below 50 C. Fabric must always be run at temperatures of 50 C or higher. Cool at a gradient of not more than 1 C per minute to prevent hydro plastic creasing.
Pre-treatmentCausticising Causticisation modifies the viscose fibre surface or skin to enable more rapid diffusion of dye into the fibre. Benefits are therefore more obvious in printing than in dyeing, where long diffusion times are employed, and with selected reactive dyes, yield gains of up to 50% are possible. Typical conditions for pure viscose are treatment with 6 - 8 B caustic soda at 25 - 30 C for at least 2 minutes followed by low tension washing with boiling water to assist the rapid removal of alkali. Pad-Batch processing is popular although dedicated continuous plant, employing a scray or conveyor for tensionless swelling and reaction, is preferable. Liquor pick-up of about 120% sho